Enhancement of GaAs solar cell efficiency by type-II GaSb quantum dots located outside of the depletion region A. Kechiantz*, &, A. Afanasev*, J.-L. Lazzari** *
Department of Physics, The George Washington University, 725 21st Street, NW, Washington, DC, 20052, USA; [email protected]
; [email protected]
** Centre Interdisciplinaire de Nanoscience de Marseille, CINaM, UMR 7325 CNRS – Aix-Marseille Université, Campus de Luminy, Case 913, 163 Avenue de Luminy, 13288 Marseille Cedex 9, France; [email protected]
& On leave of absence: Institute of Radiophysics and Electronics, National Academy of Sciences, 1 Brothers Alikhanyan st., Ashtarak 0203, Armenia; [email protected]
ABSTRACT We present a model of a new GaAs intermediate band (IB) solar cell with strained GaSb/GaAs type-II quantum dot (QD) absorber. This absorber is placed within the pdoped part of the cell such that it is spatially separated from the depletion region. We use the continuity equations along with the detailed balance principle and take into consideration the non-radiative recombination through IBstates to calculate both photocurrents and conversion efficiency of the IB cell. Our calculation shows that the newly proposed design may increase the efficiency of GaAs solar cells from 30% to 50% in response to concentration of sunlight from 1-sun to 500-sun. Noteworthy, though nonradiative recombination in QDs degrades the efficiency, it is still above the Shockley-Queisser limit by 5% to 10%. Keywords: intermediate band, quantum dot, GaAs/GaSb, solar cell, two-photon absorption
it showed that, in principle, the two-photon absorption allows to achieve 63% conversion efficiency in IB solar cells, which is much more than the Shockley-Queisser limit, 37%. However, the experiments have shown that extrinsic IB states, for instance, formed by artificial QDs imbedded in the depletion region of p-n-junction, facilitate electron-hole recombination . The latter dramatically increases the dark current and reduces the open circuit voltage of IB solar cells. In this report we present a model of a new GaAs IB solar cell with strained GaSb type-II QD absorber. This absorber is placed within the p-doped part of the cell such that it is spatially separated from the depletion region. We use the continuity equations along with the detailed balance principle and take into consideration non-radiative recombination through IB-states to calculate both photocurrents and conversion efficiency of the proposed IB cell.
2 TYPE-II QD ABSORBER
The well-developed economies aim to partially substitute their production of electricity starting from oil or nuclear origin with that of ecologically clean renewable sources like solar energy for reducing their dependence on oil- and uranium-producing nations. This makes imperative the development of third generation solar cells with higher efficiencies and lower costs. Sustained progress in development of these solar cells is firmly connected with involvement of nanotechnology as well as new ideas and physical effects into photovoltaics. In 1997, A. Luque and A. Marti offered to involve the effect of two-photon absorption to the generation of additional photocurrent in semiconductor single-junction solar cells . For enforcing this non-linear optical effect, they suggested two-photon resonant absorption via intermediate band (IB) electronic states embedded into the absorber. The effect benefits from concentration of incoming light. This work attracted much attention because
The depletion region is the most sensitive part of solar cells. We already showed that the built-in field of depletion region might facilitate recombination through QD IB electronic states . We also showed that spatial separation of IB-states from the depletion region adds more flexibility to the cell design in sense of improving the device characteristics . In particular, the separation eliminates dark current leakage through IB-states. It may also limit recombination through IB-states so much that moderate concentration of incoming sunlight may essentially increase the additional photocurrent generated by the two-photon resonant absorption in QDs. The key idea of the proposed IB solar cell is spatial separation of the type-II QD absorber of sub-band gap photons from the depletion region of ideal p-n-junction. The separation is illustrated in Figure 1 of the energy band diagram. A thin p+-doped AlxGa1-xAs buffer layer grown on an n+-doped GaAs substrate separates the QD absorber from the p+-doped AlxGa1-xAs cap layer. The QD absorber
is an epitaxial stack comprising GaSb strained QD layers alternating with p-doped AlxGa1-xAs spacers.
conduction band of absorber as shown in Figure 2.
p –AlGaAs Spacer CB
1 − 𝑒𝑥𝑝
!! !!!!" !"
where 𝜓 𝑥 is the conduction band edge bending, 𝜓! is the edge in the buffer, 𝜓! is the edge in the absorber, 𝑁! and 𝐿!"# are the doping and the Debye length in absorber. Due to the type-II misalignment of energy bands shown in Figure 1, conduction band electrons also face 𝜀!" offsetbarrier that spatially separates them from holes confined in QDs. Such spatial separation slows down the non-radiative recombination lifetime of conduction band electrons with holes confined in QDs. In GaSb/GaAs strained type-II QD system, the lifetime becomes 10 𝑛𝑠 . It is important that the 𝜀!" offset-barriers do not limit electron diffusion in
Figure 2. A schematic picture of the conduction band in absorber of the proposed solar cell. GaSb type-II QDs are sandwiched between p-doped AlxGa1-xAs spacer layers so that electrons can pass between QDs. Illumination with concentrated sunlight changes the band banding and splits the Fermi level of proposed IB solar cell. The energy band diagram shown in Figure 3 displays the change in the band bending and quasi-Fermi levels of mobile electrons in the conduction band 𝐹! , mobile holes in the valence band 𝐹! , and the holes confined in QDs 𝐹! = 𝐹! + 𝜇! . The red dashed arrows denote the photon absorptions resulting in electron-transfers to higher energy states.
εG < ħω! εQ + µQ< ħω1